Optics Communications 282 (2009) 661–665

Contents lists available at ScienceDirect

Optics Communications journal homepage: www.elsevier.com/locate/optcom

Optical response of small-diameter semiconducting carbon nanotubes under exciton–surface-plasmon coupling I.V. Bondarev a,*, K. Tatur b, L.M. Woods b a b

Physics Department, North Carolina Central University, 1801 Fayetteville Str., Durham, NC 27707, USA Physics Department, University of South Florida, 4202 E.Fowler Ave., Tampa, FL 33620, USA

a r t i c l e

i n f o

Article history: Received 4 June 2008 Received in revised form 15 October 2008 Accepted 30 October 2008

PACS: 78.40.Ri 73.22.f 73.63.Fg 78.67.Ch

a b s t r a c t We analyze the optical response of small-diameter ([1 nm) semiconducting carbon nanotubes under the exciton–surface-plasmon coupling. Calculated optical absorption lineshapes exhibit the signiﬁcant line (Rabi) splitting 0.1–0.3 eV as the exciton energy is tuned to the nearest interband surface plasmon resonance of the nanotube so that the mixed strongly coupled surface plasmon–exciton excitations are formed. We discuss possible ways to bring the exciton in resonance with the surface plasmon. The exciton–plasmon Rabi splitting effect we predict here for an individual carbon nanotube is close in its magnitude to that previously reported for hybrid plasmonic nanostructures artiﬁcially fabricated of organic semiconductors deposited on metallic ﬁlms. We believe this effect may be used for the development of carbon nanotube based tunable optoelectronic device applications in areas such as nanophotonics and cavity quantum electrodynamics. Ó 2008 Elsevier B.V. All rights reserved.

Single-walled carbon nanotubes (CNs) are quasi-one-dimensional (1D) cylindrical wires consisting of graphene sheets rolledup into cylinders with diameters 1–10 nm and lengths 1– 104 lm [1–3]. CNs are shown to be useful for miniaturized electronic, electromechanical, chemical and scanning probe devices and as materials for macroscopic composites [4]. The area of their potential applications has been recently expanded towards nanophotonics and optoelectronics [5,6] after the experimental demonstration of controllable single-atom incapsulation into singlewalled CNs [7,8]. For pristine (undoped) single-walled CNs, the numerical calculations predicting large exciton binding energies (0.3–0.6 eV) in semiconducting CNs [9–11] and even in some small-diameter (0.5 nm) metallic CNs [12], followed by the results of various measurements of the excitonic photoluminescence [13–16], have become available. These works, together with other reports investigating the role of effects such as intrinsic defects [15], exciton– phonon interactions [16–19], external magnetic and electric ﬁelds [20,21], reveal the variety and complexity of the intrinsic optical properties of carbon nanotubes. One of us have reported earlier the interactions between excitonic states and surface electromagnetic (EM) ﬂuctuations to result in the strong exciton–surface-plasmon coupling in small-diameter ([1 nm) semiconducting single-walled CNs [22]. The reason is, due to the nanotube quasi-one-dimensionality, the exciton transi* Corresponding author. E-mail address: [email protected] (I.V. Bondarev). 0030-4018/$ - see front matter Ó 2008 Elsevier B.V. All rights reserved. doi:10.1016/j.optcom.2008.10.074

tion dipole moment matrix element and the quasi-momentum vector are directed predominantly along the CN axis (the longitudinal exciton). This prevents the exciton from the electric dipole coupling to the transversely polarized surface EM modes of the nanotube as they propagate predominantly along the CN axis with their electric vectors orthogonal to the propagation direction. The longitudinally polarized surface EM modes are generated by the electronic Coulomb potential (see, e.g., Ref. [23]), and therefore represent the CN surface plasmon excitations. These have their electric vectors directed along the propagation direction. They do couple to the longitudinal excitons on the CN surface [22]. Such modes were observed in Ref. [24] to occur in the same energy range of 1 eV where the exciton excitation energies are located in small-diameter ([1 nm) semiconducting CNs [25,26]. They are the weakly-dispersive interband plasmon modes [27] similar to the intersubband plasmon modes in quantum wells [28]. Here we analyze the optical response of small-diameter semiconducting CNs under the strong exciton–surface-plasmon coupling. The calculated optical absorption lineshapes of the (11, 0) and (10, 0) CNs exhibit the signiﬁcant line (Rabi) splitting effect 0.1 eV as the exciton energy is tuned to the nearest interband surface plasmon resonance of the nanotube. This result is particularly interesting since it reveals the fundamental EM phenomenon – the strong exciton–plasmon coupling – in an individual quasione-dimensional (1D) nanostructure, a carbon nanotube, as opposed to various artiﬁcially fabricated hybrid plasmonic nanostructures, such as dye molecules in organic polymers deposited on metallic ﬁlms [29], semiconductor quantum dots coupled to metal-

662

I.V. Bondarev et al. / Optics Communications 282 (2009) 661–665

lic nanoparticles [30], or nanowires [31], where semiconductor material carries the exciton and metal carries the plasmon. The energy hxl ðkÞ of the coupled exciton–surface-plasmon excitation of branch l ð¼ 1; 2Þ is given by the integral dispersion relation [22], which is written in the dimensionless form as follows:

x2l e2f

ef 2p

Z

1

dx 0

xCf0 ðxÞqðxÞ ¼ 0: x2l x2

ð1Þ Re

Here,

x¼

hx ; 2c0

xl ¼

h xl ðkÞ ; 2c0

ef ¼

Ef ðkÞ 2c0

ð2Þ

with c0 ¼ 2:7 eV being the carbon nearest neighbor overlap integral entering the CN surface axial conductivity rzz (the CN axis is assigned to be the z-axis of the cylindrical coordinate system we use, and we neglect much smaller azimuthal conductivity component ruu in our model). The total energy Ef ðkÞ of the f-internal-state exciton with the quasi-momentum k ¼ fku ; kz g, where kz is continuous and ku is quantized due to the transverse conﬁnement effect, is given by 2 2

Ef ðkÞ ¼ EðfexcÞ ðku Þ þ

kz h 2M ex

ð3Þ

with the ﬁrst term representing the excitation energy, ðf Þ EðfexcÞ ðku Þ ¼ Eg ðku Þ þ Eb , of the f-internal-state exciton with the (negðf Þ ative) binding energy Eb , created via the interband transition with the band gap Eg ðku Þ ¼ ee ðku Þ þ eh ðku Þ, where ee;h are transversely quantized azimuthal electron–hole subbands (see the schematic in Fig. 1). The second term represents the kinetic energy of the translational longitudinal movement of the exciton with the effective mass Mex ¼ me þ mh , where me and mh are the electron and hole effective masses, respectively. The function

Cf0 ðxÞ ¼

2 f 4jdz j2 x3 2c0 3hc3 h

ð4Þ

represents the (dimensionless) exciton spontaneous decay rate. P f ^ n Þ jf i (summation over Here, c is the speed of light and dz ¼ n h0jðd z carbon atoms) is the longitudinal exciton transition dipole moment matrix element. The function

qðxÞ ¼

3S0 4paR2CN

Re

1

r zz ðxÞ

stands for the surface plasmon density of states (DOS) which is responsible for the exciton decayprate due to the coupling ﬃﬃﬃ variation 2 to plasmon modes. Here, S0 ¼ ð3 3=4Þb with b ¼ 1:42 Å being the hc ¼ 1=137 is the ﬁnecarbon–carbon interatomic distance, a ¼ e2 = zz ¼ 2ph rzz =e2 structure constant, RCN is the nanotube radius, and r is the dimensionless CN surface axial conductivity per unit length. Note that the conductivity factor in Eq. (5) equals

ð5Þ

Fig. 1. Schematic of the transversely quantized azimuthal electron–hole subbands (left), and the ﬁrst-interband ground-internal-state exciton energy (right) in a smalldiameter semiconducting carbon nanotube. See text for notations.

1 4ac h 1 ¼ Im RCN 2c0 x r zz ðxÞ zz ðxÞ 1

ð6Þ

in view of Eq. (2) and the formula rzz ¼ ixðzz 1Þ=4pSqT representing the Drude relation for CNs, where zz is the longitudinal dielectric function, S and qT are the surface area of the tubule and the number of tubules per unit volume, respectively [32–35]. This relates very closely the surface plasmon DOS function Eq. (5) to the loss function Imð1=Þ measured in electron energy loss spectroscopy (EELS) experiments to determine the properties of collective electronic excitations in solids [24]. zz ðxÞ Fig. 2 shows the low-energy behaviors of the functions r zz ðxÞ for the (11, 0) and (10, 0) CNs (RCN ¼ 0:43 nm and Re½1=r and 0:39 nm, respectively) we study here. We obtained them numerically as follows. First, we adapt the nearest-neighbor non-orthogonal tight-binding approach [36] to determine the realistic band structure of each CN. Then, the room-temperature longitudinal dielectric functions zz are calculated within the random-phase approximation [37,38], which are then converted into zz by means of the Drude relation. Electronic the conductivities r dissipation processes are included in our calculations within the relaxation-time approximation (electron scattering length of 130RCN was used [18]). We did not include excitonic many-electron correlations, however, as they mostly affect the real conduc zz Þ which is responsible for the CN optical absorption tivity Reðr zz Þ represent[10,12,39], whereas we are interested here in Reð1=r ing the surface plasmon DOS according to Eq. (5). This function is zz ðxÞ ¼ 0 and only non-zero when the two conditions, Im½r zz ðxÞ ! 0, are fulﬁlled simultaneously [27,28,37]. These result Re½r zz Þ as is seen in Fig. 2. in the peak structure of the function Reð1=r It is also seen from the comparison of Fig. 2b with Fig. 2a that the peaks broaden as the CN diameter decreases. This is consistent with the stronger hybridization effects in smaller-diameter CNs [40]. Left panels in Fig. 3a and b show the lowest-energy plasmon DOS resonances calculated for the (11, 0) and (10, 0) CNs as given by the function qðxÞ in Eq. (5). The corresponding fragments of zz ðxÞ are also shown there. In all zz ðxÞ and Im½r the functions Re½r graphs the lower dimensionless energy limits are set up to be equal to the lowest bright exciton excitation energy [Eexc ¼ 1:21 eV (x ¼ 0:224) and 1:00 eV (x ¼ 0:185) for the (11, 0) and (10, 0) CN, respectively, as reported in Ref. [25] by directly solving the Bethe–Salpeter equation]. Peaks in qðxÞ are seen to coincide in en zz ðxÞ {or zeros of Re½zz ðxÞ}, clearly indicatergy with zeros of Im½r ing the plasmonic nature of the CN surface excitations under consideration [27,41]. They describe the surface plasmon modes associated with the transversely quantized interband electronic transitions in CNs [27]. As is seen in Fig. 3 (and in Fig. 2), the interband plasmon excitations occur in CNs slightly above the ﬁrst bright exciton excitation energy [39], which is a unique feature of the complex dielectric response function – the consequence of the general Kramers–Krönig relation [42]. We further take advantage of the sharp peak structure of qðxÞ and solve the dispersion Eq. (1) for xl analytically using the Lorentzian approximation

qðxÞ

qðxp ÞDx2p ðx xp Þ2 þ Dx2p

:

ð7Þ

I.V. Bondarev et al. / Optics Communications 282 (2009) 661–665

663

Fig. 2. (a) and (b) Calculated (see text) dimensionless axial surface conductivities for the (11, 0) and (10, 0) nanotubes. Dimensionless energy is deﬁned as ½Energy=2c0 , according to Eq. (2).

Fig. 3. (a) and (b) Surface plasmon DOS and conductivities (left panels), and lowest bright exciton dispersion when coupled to plasmons (right panels) in the (11, 0) and (10, 0) CN, respectively. Dimensionless energy is deﬁned as ½Energy=2c0 , according to Eq. (2). See text for dimensionless quasi-momentum.

Here, xp and Dxp are, respectively, the position and the half-widthat-half-maximum of the plasmon resonance closest to the lowest bright exciton excitation energy in the same nanotube (as shown in the left panels of Fig. 3). The integral in Eq. (1) then simpliﬁes to the form

1 2p

Z 0

1

dx

Z xCf0 ðxÞqðxÞ Fðxp ÞDx2p 1 dx x2l x2 x2l x2p 0 ðx xp Þ2 þ Dx2p Fðxp ÞDxp xp p ¼ 2 arctan þ xl x2p Dxp 2

ð8Þ

with Fðxp Þ ¼ xp Cf0 ðxp Þqðxp Þ=2p. This expression is valid for all xl apart from those located in the narrow interval ðxp Dxp ; xp þ Dxp Þ in the vicinity of the plasmon resonance, provided that the resonance is sharp enough. Then, the dispersion equation becomes the biquadratic equation for xl with the following two positive solutions (the dispersion curves) of interest to us:

x1;2

sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ e2f þ x2p 1 qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ¼ ðe2f x2p Þ2 þ F p ef : 2 2

ð9Þ

Here, F p ¼ 4Fðxp ÞDxp ðp Dxp =xp Þ, and the arctan-function of Eq. (8) is expanded into series to linear terms in Dxp =xp 1. The dispersion curves Eq. (9) are shown in the right panels in Fig. 3a and b as functions of the dimensionless longitudinal quasi-momentum. In these calculations, we estimated the interband transition matrix element in Cf0 ðxp Þ [Eq. (4)] from the equation f hk3 =4srad jdz j2 ¼ 3 ex according to Hanamura’s general theory of the exciton radiative decay in spatially conﬁned systems [43], where srad h=E with ex is the exciton intrinsic radiative lifetime, and k ¼ 2pc E being the exciton total energy given in our case by Eq. (3). For zigzag-type CNs we here consider, the ﬁrst Brillouin zone of the lonh=3b 6 hkz 6 2p h=3b gitudinal quasi-momentum is given by 2p [1,2]. The total energy of the ground-internal-state exciton can h=3bÞ2 t2 =2Mex with 1 6 t 6 1 then be written as E ¼ Eexc þ ð2p representing the dimensionless longitudinal quasi-momentum. In our calculations we used the lowest bright exciton parameters and 19:1 ps, Eexc ¼ 1:21 eV and 1:00 eV, srad ex ¼ 14:3 ps Mex ¼ 0:44m0 and 0:19m0 (m0 is the free-electron mass) for the (11, 0) CN and (10, 0) CN, respectively, as reported in Ref. [25] by directly solving the Bethe–Salpeter equation.

664

I.V. Bondarev et al. / Optics Communications 282 (2009) 661–665

Fig. 4. (a) and (b) Exciton absorption lineshapes as the exciton energies are tuned to the nearest plasmon resonance energies (vertical dashed lines here; see Fig. 3, left panels) in the (11, 0) and (10, 0) CN, respectively. Dimensionless energy is deﬁned as ½Energy=2c0 , according to Eq. (2).

Both graphs in the right panels in Fig. 3 are seen to demonstrate a clear anticrossing behavior with the (Rabi) energy splitting 0.1 eV. This indicates the formation of the strongly coupled surface plasmon–exciton excitations in the nanotubes under consideration. It is important to realize that here we deal with the strong exciton–plasmon interaction supported by an individual quasi-1D nanostructure – a single-walled (small-diameter) semiconducting carbon nanotube, as opposed to the artiﬁcially fabricated metal– semiconductor nanostructures studied previously [29–31] where the metallic component normally carries the plasmon and the semiconducting one carries the exciton. It is also important that the effect comes not only from the height but also from the width of the plasmon resonance as is seen from the deﬁnition of the F p factor in Eq. (9). In other words, as long as the plasmon resonance is sharp enough (which is always the case for interband plasmons), so that the Lorentzian approximation Eq. (7) applies, the effect is determined by the area under the plasmon peak in the DOS function Eq. (5) rather then by the peak height as one would expect. We are now in a position to derive the exciton absorption lineshape function. To do that, we follow the optical absorption lineshape theory that one of us developed recently for atomically doped CNs [5]. In doing so, we take into account the exciton–phonon scattering in the relaxation time approximation. The (dimensionless) exciton absorption lineshape function IðxÞ in the vicinity of the plasmon resonance is then of the form

IðxÞ ¼

I0 ðxp Þ½ðx ef Þ2 þ Dx2p 2

½ðx ef Þ X 2f =42 þ ðx ef Þ2 ðDx2p þ De2f Þ

;

ð10Þ

pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ where I0 ðxp Þ ¼ Cf0 ðxp Þqðxp Þ=2p, X f ¼ 4pDxp I0 ðxp Þ, and Def ¼ h=2c0 sph ð< Dxp Þ is the exciton energy broadening due to the pho non scattering with the relaxation time sph . The calculated exciton absorption lineshapes for the CNs under consideration are shown in Fig. 4a and b as the exciton energies are tuned to the nearest plasmon resonances. We used sph ¼ 30 fs as reported in Ref. [17]. The line (Rabi) splitting effect is seen to be 0.1–0.3 eV, indicating the strong exciton–plasmon coupling with the formation of the mixed surface plasmon–exciton excitations. The splitting is larger in the smaller diameter nanotubes, and is not masked by the exciton–phonon scattering. Thus, we have shown the strong exciton–surface-plasmon coupling effect with the characteristic exciton absorption line (Rabi) splitting 0.1–0.3 eV in small-diameter ([1 nm) semiconducting CNs. This is almost as large as the typical exciton binding energies in such CNs (0.3–0.8 eV [9–11,14]), and of the same order of magnitude as the exciton–plasmon Rabi splitting in organic semiconductors (180 meV [29]). Also, this is much larger than the exciton–polariton Rabi splitting in semiconductor microcavities (140–400 leV [44–46]), or the exciton–plasmon Rabi splitting

in hybrid semiconductor–metal nanoparticle molecules [30]. However, the formation of the strongly coupled exciton–plasmon states is only possible if the exciton total energy is in resonance with the energy of an interband surface plasmon mode. The exciton energy might be tuned to the nearest plasmon resonance in ways used for the excitons in semiconductor quantum microcavities – thermally (by elevating sample temperature) [44–46], and/or electrostatically [47–50] (via the quantum conﬁned Stark effect with an external electrostatic ﬁeld applied perpendicular to the CN axis). The two possibilities inﬂuence the different degrees of freedom of the quasi-1D exciton – the (longitudinal) kinetic energy and the excitation energy, respectively [see Eq. (3)]. In the latter case, plasmon and exciton resonances both shift to the red due to the decrease in Eg as the ﬁeld increases [48]. However, the exciton shift is approximately twice as less due to the decrease in jEb j (see Ref. [48]), which is enough for the resonance to occur in view of the large jEb j contribution 0:5Eexc in small-diameter CNs [9–11,14]. This effect may be used for the development of CN based tunable optoelectronic device applications in areas such as nanophotonics and cavity quantum electrodynamics. Acknowledgements The work is supported by NSF (Grant Nos. ECS-0631347 and HRD-0833184). K.T. and L.M.W. are supported by DOE (Grant No. DE-FG02-06ER46297). I.V.B. acknowledges fruitful discussions with Alexander Govorov and Jonathan Finley. References [1] R. Saito, G. Dresselhaus, M.S. Dresselhaus, Science of Fullerens and Carbon Nanotubes, Imperial College Press, London, 1998. [2] H. Dai, Surf. Sci. 500 (2002) 218. [3] L.X. Zheng, M.J. O’Connell, S.K. Doorn, X.Z. Liao, Y.H. Zhao, E.A. Akhadov, M.A. Hoffbauer, B.J. Roop, Q.X. Jia, R.C. Dye, D.E. Peterson, S.M. Huang, J. Liu, Y.T. Zhu, Nat. Mater. 3 (2004) 673. [4] R.H. Baughman, A.A. Zakhidov, W.A. de Heer, Science 297 (2002) 787. [5] I.V. Bondarev, B. Vlahovic, Phys. Rev. B 74 (2006) 073401. [6] I.V. Bondarev, B. Vlahovic, Phys. Rev. B 75 (2007) 033402. [7] G.-H. Jeong, A.A. Farajian, R. Hatakeyama, T. Hirata, T. Yaguchi, K. Tohji, H. Mizuseki, Y. Kawazoe, Phys. Rev. B 68 (2003) 075410. [8] G.-H. Jeong, A.A. Farajian, T. Hirata, R. Hatakeyama, K. Tohji, T.M. Briere, H. Mizuseki, Y. Kawazoe, Thin Solid Films 435 (2003) 307. [9] T. Pedersen, Phys. Rev. B 67 (2003) 073401. [10] T. Pedersen, Carbon 42 (2004) 1007. [11] R.B. Capaz, C.D. Spataru, S. Ismail-Beigi, S.G. Louie, Phys. Rev. B 74 (2006) 121401. R. [12] C.D. Spataru, S. Ismail-Beigi, L.X. Benedict, S.G. Louie, Phys. Rev. Lett. 92 (2004) 077402. [13] F. Wang, G. Dukovic, L.E. Brus, T.F. Heinz, Phys. Rev. Lett. 92 (2004) 177401. [14] F. Wang, G. Dukovic, L.E. Brus, T.F. Heinz, Science 308 (2005) 838. [15] A. Hagen, M. Steiner, M.B. Raschke, C. Lienau, T. Hertel, H. Qian, A.J. Meixner, A. Hartschuh, Phys. Rev. Lett. 95 (2005) 197401. [16] F. Plentz, H.B. Ribeiro, A. Jorio, M.S. Strano, M.A. Pimenta, Phys. Rev. Lett. 95 (2005) 247401.

I.V. Bondarev et al. / Optics Communications 282 (2009) 661–665 [17] V. Perebeinos, J. Tersoff, Ph. Avouris, Phys. Rev. Lett. 94 (2005) 027402. [18] M. Lazzeri, S. Piscanec, F. Mauri, A.C. Ferrari, J. Robertson, Phys. Rev. Lett. 95 (2005) 236802. [19] S. Piscanec, M. Lazzeri, J. Robertson, A. Ferrari, F. Mauri, Phys. Rev. B 75 (2007) 035427. [20] S. Zaric, G.N. Ostojic, J. Shaver, J. Kono, O. Portugall, P.H. Frings, G.L.J.A. Rikken, M. Furis, S.A. Crooker, X. Wei, V.C. Moore, R.H. Hauge, R.E. Smalley, Phys. Rev. Lett. 96 (2006) 016406. [21] V. Perebeinos, Ph. Avouris, Nano Lett. 7 (2007) 609. [22] I.V. Bondarev, H. Qasmi, Physica E 40 (2008) 2365. [23] L.D. Landau, E.M. Lifshits, The Classical Theory of Fields, Pergamon, New York, 1975. [24] T. Pichler, M. Knupfer, M.S. Golden, J. Fink, A. Rinzler, R.E. Smalley, Phys. Rev. Lett. 80 (1998) 4729. [25] C.D. Spataru, S. Ismail-Beigi, R.B. Capaz, S.G. Louie, Phys. Rev. Lett. 95 (2005) 247402. [26] Y.-Z. Ma, C.D. Spataru, L. Valkunas, S.G. Louie, G.R. Fleming, Phys. Rev. B 74 (2006) 085402. [27] K. Kempa, P.R. Chura, in: L. Liz-Marzan, M. Giersig (Eds.), Special edition of the Kluwer Academic Press Journal, 2002. [28] K. Kempa, D. Broido, C. Beckwith, J. Cen, Phys. Rev. B 40 (1989) 8385. [29] J. Bellessa, C. Bonnand, J.C. Plenet, J. Mugnier, Phys. Rev. Lett. 93 (2004) 036404. [30] W. Zhang, A.O. Govorov, G.W. Bryant, Phys. Rev. Lett. 97 (2006) 146804. [31] Y. Fedutik, V.V. Temnov, O. Schöps, U. Woggon, M.V. Artemyev, Phys. Rev. Lett. 99 (2007) 136802. [32] I.V. Bondarev, Ph. Lambin, Phys. Rev. B 70 (2004) 035407; I.V. Bondarev, Ph. Lambin, Phys. Lett. A 328 (2004) 235.

665

[33] I.V. Bondarev, Ph. Lambin, Phys. Rev. B 72 (2005) 035451; I.V. Bondarev, Ph. Lambin, Solid State Commun. 132 (2004) 203. [34] I.V. Bondarev, Ph. Lambin, in: Trends in Nanotubes Research, Nova Science, NY, 2006, pp. 139–183 (Chapter 6). [35] S. Tasaki, K. Maekawa, T. Yamabe, Phys. Rev. B 57 (1998) 9301. [36] V.N. Popov, L. Henrard, Phys. Rev. B 70 (2004) 115407. [37] M.F. Lin, D.S. Chuu, K.W.-K. Shung, Phys. Rev. B 56 (1997) 1430. [38] H. Ehrenreich, M.H. Cohen, Phys. Rev. 115 (1959) 786. [39] T. Ando, J. Phys. Soc. Jpn. 74 (2005) 777. [40] X. Blase, L.X. Benedict, E.L. Shirley, S.G. Louie, Phys. Rev. Lett. 72 (1994) 1878. [41] K. Kempa, Phys. Rev. B 66 (2002) 195406. [42] W. Vogel, D.-G. Welsch, Quantum Optics, Wiley-VCH, NY, 2006. p. 337 (Chapter 10). [43] E. Hanamura, Phys. Rev. B 38 (1998) 1228. [44] J.P. Reithmaier, G. Se ß k, A. Löfﬂer, C. Hofmann, S. Kuhn, S. Reitzenstein, L.V. Keldysh, V.D. Kulakovskii, T.L. Reinecke, A. Forchel, Nature 432 (2004) 197. [45] T. Yoshie, A. Scherer, J. Hendrickson, G. Khitrova, H.M. Gibbs, G. Rupper, C. Ell, O.B. Shchekin, D.G. Deppe, Nature 432 (2004) 200. [46] E. Peter, P. Senellart, D. Martrou, A. Lemaître, J. Hours, J.M. Gérard, J. Bloch, Phys. Rev. Lett. 95 (2005) 067401. [47] D.A.B. Miller, D.S. Chemla, T.C. Damen, A.C. Gossard, W. Wiegmann, T.H. Wood, C.A. Burrus, Phys. Rev. Lett. 53 (1984) 2173. [48] D.A.B. Miller, D.S. Chemla, T.C. Damen, A.C. Gossard, W. Wiegmann, T.H. Wood, C.A. Burrus, Phys. Rev. B 32 (1985) 1043. [49] A. Zrenner, E. Beham, S. Stuﬂer, F. Findeis, M. Bichler, G. Abstreiter, Nature 418 (2002) 612. [50] H.J. Krenner, E.C. Clark, T. Nakaoka, M. Bichler, C. Scheurer, G. Abstreiter, J.J. Finley, Phys. Rev. Lett. 97 (2006) 076403.

Contents lists available at ScienceDirect

Optics Communications journal homepage: www.elsevier.com/locate/optcom

Optical response of small-diameter semiconducting carbon nanotubes under exciton–surface-plasmon coupling I.V. Bondarev a,*, K. Tatur b, L.M. Woods b a b

Physics Department, North Carolina Central University, 1801 Fayetteville Str., Durham, NC 27707, USA Physics Department, University of South Florida, 4202 E.Fowler Ave., Tampa, FL 33620, USA

a r t i c l e

i n f o

Article history: Received 4 June 2008 Received in revised form 15 October 2008 Accepted 30 October 2008

PACS: 78.40.Ri 73.22.f 73.63.Fg 78.67.Ch

a b s t r a c t We analyze the optical response of small-diameter ([1 nm) semiconducting carbon nanotubes under the exciton–surface-plasmon coupling. Calculated optical absorption lineshapes exhibit the signiﬁcant line (Rabi) splitting 0.1–0.3 eV as the exciton energy is tuned to the nearest interband surface plasmon resonance of the nanotube so that the mixed strongly coupled surface plasmon–exciton excitations are formed. We discuss possible ways to bring the exciton in resonance with the surface plasmon. The exciton–plasmon Rabi splitting effect we predict here for an individual carbon nanotube is close in its magnitude to that previously reported for hybrid plasmonic nanostructures artiﬁcially fabricated of organic semiconductors deposited on metallic ﬁlms. We believe this effect may be used for the development of carbon nanotube based tunable optoelectronic device applications in areas such as nanophotonics and cavity quantum electrodynamics. Ó 2008 Elsevier B.V. All rights reserved.

Single-walled carbon nanotubes (CNs) are quasi-one-dimensional (1D) cylindrical wires consisting of graphene sheets rolledup into cylinders with diameters 1–10 nm and lengths 1– 104 lm [1–3]. CNs are shown to be useful for miniaturized electronic, electromechanical, chemical and scanning probe devices and as materials for macroscopic composites [4]. The area of their potential applications has been recently expanded towards nanophotonics and optoelectronics [5,6] after the experimental demonstration of controllable single-atom incapsulation into singlewalled CNs [7,8]. For pristine (undoped) single-walled CNs, the numerical calculations predicting large exciton binding energies (0.3–0.6 eV) in semiconducting CNs [9–11] and even in some small-diameter (0.5 nm) metallic CNs [12], followed by the results of various measurements of the excitonic photoluminescence [13–16], have become available. These works, together with other reports investigating the role of effects such as intrinsic defects [15], exciton– phonon interactions [16–19], external magnetic and electric ﬁelds [20,21], reveal the variety and complexity of the intrinsic optical properties of carbon nanotubes. One of us have reported earlier the interactions between excitonic states and surface electromagnetic (EM) ﬂuctuations to result in the strong exciton–surface-plasmon coupling in small-diameter ([1 nm) semiconducting single-walled CNs [22]. The reason is, due to the nanotube quasi-one-dimensionality, the exciton transi* Corresponding author. E-mail address: [email protected] (I.V. Bondarev). 0030-4018/$ - see front matter Ó 2008 Elsevier B.V. All rights reserved. doi:10.1016/j.optcom.2008.10.074

tion dipole moment matrix element and the quasi-momentum vector are directed predominantly along the CN axis (the longitudinal exciton). This prevents the exciton from the electric dipole coupling to the transversely polarized surface EM modes of the nanotube as they propagate predominantly along the CN axis with their electric vectors orthogonal to the propagation direction. The longitudinally polarized surface EM modes are generated by the electronic Coulomb potential (see, e.g., Ref. [23]), and therefore represent the CN surface plasmon excitations. These have their electric vectors directed along the propagation direction. They do couple to the longitudinal excitons on the CN surface [22]. Such modes were observed in Ref. [24] to occur in the same energy range of 1 eV where the exciton excitation energies are located in small-diameter ([1 nm) semiconducting CNs [25,26]. They are the weakly-dispersive interband plasmon modes [27] similar to the intersubband plasmon modes in quantum wells [28]. Here we analyze the optical response of small-diameter semiconducting CNs under the strong exciton–surface-plasmon coupling. The calculated optical absorption lineshapes of the (11, 0) and (10, 0) CNs exhibit the signiﬁcant line (Rabi) splitting effect 0.1 eV as the exciton energy is tuned to the nearest interband surface plasmon resonance of the nanotube. This result is particularly interesting since it reveals the fundamental EM phenomenon – the strong exciton–plasmon coupling – in an individual quasione-dimensional (1D) nanostructure, a carbon nanotube, as opposed to various artiﬁcially fabricated hybrid plasmonic nanostructures, such as dye molecules in organic polymers deposited on metallic ﬁlms [29], semiconductor quantum dots coupled to metal-

662

I.V. Bondarev et al. / Optics Communications 282 (2009) 661–665

lic nanoparticles [30], or nanowires [31], where semiconductor material carries the exciton and metal carries the plasmon. The energy hxl ðkÞ of the coupled exciton–surface-plasmon excitation of branch l ð¼ 1; 2Þ is given by the integral dispersion relation [22], which is written in the dimensionless form as follows:

x2l e2f

ef 2p

Z

1

dx 0

xCf0 ðxÞqðxÞ ¼ 0: x2l x2

ð1Þ Re

Here,

x¼

hx ; 2c0

xl ¼

h xl ðkÞ ; 2c0

ef ¼

Ef ðkÞ 2c0

ð2Þ

with c0 ¼ 2:7 eV being the carbon nearest neighbor overlap integral entering the CN surface axial conductivity rzz (the CN axis is assigned to be the z-axis of the cylindrical coordinate system we use, and we neglect much smaller azimuthal conductivity component ruu in our model). The total energy Ef ðkÞ of the f-internal-state exciton with the quasi-momentum k ¼ fku ; kz g, where kz is continuous and ku is quantized due to the transverse conﬁnement effect, is given by 2 2

Ef ðkÞ ¼ EðfexcÞ ðku Þ þ

kz h 2M ex

ð3Þ

with the ﬁrst term representing the excitation energy, ðf Þ EðfexcÞ ðku Þ ¼ Eg ðku Þ þ Eb , of the f-internal-state exciton with the (negðf Þ ative) binding energy Eb , created via the interband transition with the band gap Eg ðku Þ ¼ ee ðku Þ þ eh ðku Þ, where ee;h are transversely quantized azimuthal electron–hole subbands (see the schematic in Fig. 1). The second term represents the kinetic energy of the translational longitudinal movement of the exciton with the effective mass Mex ¼ me þ mh , where me and mh are the electron and hole effective masses, respectively. The function

Cf0 ðxÞ ¼

2 f 4jdz j2 x3 2c0 3hc3 h

ð4Þ

represents the (dimensionless) exciton spontaneous decay rate. P f ^ n Þ jf i (summation over Here, c is the speed of light and dz ¼ n h0jðd z carbon atoms) is the longitudinal exciton transition dipole moment matrix element. The function

qðxÞ ¼

3S0 4paR2CN

Re

1

r zz ðxÞ

stands for the surface plasmon density of states (DOS) which is responsible for the exciton decayprate due to the coupling ﬃﬃﬃ variation 2 to plasmon modes. Here, S0 ¼ ð3 3=4Þb with b ¼ 1:42 Å being the hc ¼ 1=137 is the ﬁnecarbon–carbon interatomic distance, a ¼ e2 = zz ¼ 2ph rzz =e2 structure constant, RCN is the nanotube radius, and r is the dimensionless CN surface axial conductivity per unit length. Note that the conductivity factor in Eq. (5) equals

ð5Þ

Fig. 1. Schematic of the transversely quantized azimuthal electron–hole subbands (left), and the ﬁrst-interband ground-internal-state exciton energy (right) in a smalldiameter semiconducting carbon nanotube. See text for notations.

1 4ac h 1 ¼ Im RCN 2c0 x r zz ðxÞ zz ðxÞ 1

ð6Þ

in view of Eq. (2) and the formula rzz ¼ ixðzz 1Þ=4pSqT representing the Drude relation for CNs, where zz is the longitudinal dielectric function, S and qT are the surface area of the tubule and the number of tubules per unit volume, respectively [32–35]. This relates very closely the surface plasmon DOS function Eq. (5) to the loss function Imð1=Þ measured in electron energy loss spectroscopy (EELS) experiments to determine the properties of collective electronic excitations in solids [24]. zz ðxÞ Fig. 2 shows the low-energy behaviors of the functions r zz ðxÞ for the (11, 0) and (10, 0) CNs (RCN ¼ 0:43 nm and Re½1=r and 0:39 nm, respectively) we study here. We obtained them numerically as follows. First, we adapt the nearest-neighbor non-orthogonal tight-binding approach [36] to determine the realistic band structure of each CN. Then, the room-temperature longitudinal dielectric functions zz are calculated within the random-phase approximation [37,38], which are then converted into zz by means of the Drude relation. Electronic the conductivities r dissipation processes are included in our calculations within the relaxation-time approximation (electron scattering length of 130RCN was used [18]). We did not include excitonic many-electron correlations, however, as they mostly affect the real conduc zz Þ which is responsible for the CN optical absorption tivity Reðr zz Þ represent[10,12,39], whereas we are interested here in Reð1=r ing the surface plasmon DOS according to Eq. (5). This function is zz ðxÞ ¼ 0 and only non-zero when the two conditions, Im½r zz ðxÞ ! 0, are fulﬁlled simultaneously [27,28,37]. These result Re½r zz Þ as is seen in Fig. 2. in the peak structure of the function Reð1=r It is also seen from the comparison of Fig. 2b with Fig. 2a that the peaks broaden as the CN diameter decreases. This is consistent with the stronger hybridization effects in smaller-diameter CNs [40]. Left panels in Fig. 3a and b show the lowest-energy plasmon DOS resonances calculated for the (11, 0) and (10, 0) CNs as given by the function qðxÞ in Eq. (5). The corresponding fragments of zz ðxÞ are also shown there. In all zz ðxÞ and Im½r the functions Re½r graphs the lower dimensionless energy limits are set up to be equal to the lowest bright exciton excitation energy [Eexc ¼ 1:21 eV (x ¼ 0:224) and 1:00 eV (x ¼ 0:185) for the (11, 0) and (10, 0) CN, respectively, as reported in Ref. [25] by directly solving the Bethe–Salpeter equation]. Peaks in qðxÞ are seen to coincide in en zz ðxÞ {or zeros of Re½zz ðxÞ}, clearly indicatergy with zeros of Im½r ing the plasmonic nature of the CN surface excitations under consideration [27,41]. They describe the surface plasmon modes associated with the transversely quantized interband electronic transitions in CNs [27]. As is seen in Fig. 3 (and in Fig. 2), the interband plasmon excitations occur in CNs slightly above the ﬁrst bright exciton excitation energy [39], which is a unique feature of the complex dielectric response function – the consequence of the general Kramers–Krönig relation [42]. We further take advantage of the sharp peak structure of qðxÞ and solve the dispersion Eq. (1) for xl analytically using the Lorentzian approximation

qðxÞ

qðxp ÞDx2p ðx xp Þ2 þ Dx2p

:

ð7Þ

I.V. Bondarev et al. / Optics Communications 282 (2009) 661–665

663

Fig. 2. (a) and (b) Calculated (see text) dimensionless axial surface conductivities for the (11, 0) and (10, 0) nanotubes. Dimensionless energy is deﬁned as ½Energy=2c0 , according to Eq. (2).

Fig. 3. (a) and (b) Surface plasmon DOS and conductivities (left panels), and lowest bright exciton dispersion when coupled to plasmons (right panels) in the (11, 0) and (10, 0) CN, respectively. Dimensionless energy is deﬁned as ½Energy=2c0 , according to Eq. (2). See text for dimensionless quasi-momentum.

Here, xp and Dxp are, respectively, the position and the half-widthat-half-maximum of the plasmon resonance closest to the lowest bright exciton excitation energy in the same nanotube (as shown in the left panels of Fig. 3). The integral in Eq. (1) then simpliﬁes to the form

1 2p

Z 0

1

dx

Z xCf0 ðxÞqðxÞ Fðxp ÞDx2p 1 dx x2l x2 x2l x2p 0 ðx xp Þ2 þ Dx2p Fðxp ÞDxp xp p ¼ 2 arctan þ xl x2p Dxp 2

ð8Þ

with Fðxp Þ ¼ xp Cf0 ðxp Þqðxp Þ=2p. This expression is valid for all xl apart from those located in the narrow interval ðxp Dxp ; xp þ Dxp Þ in the vicinity of the plasmon resonance, provided that the resonance is sharp enough. Then, the dispersion equation becomes the biquadratic equation for xl with the following two positive solutions (the dispersion curves) of interest to us:

x1;2

sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ e2f þ x2p 1 qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ¼ ðe2f x2p Þ2 þ F p ef : 2 2

ð9Þ

Here, F p ¼ 4Fðxp ÞDxp ðp Dxp =xp Þ, and the arctan-function of Eq. (8) is expanded into series to linear terms in Dxp =xp 1. The dispersion curves Eq. (9) are shown in the right panels in Fig. 3a and b as functions of the dimensionless longitudinal quasi-momentum. In these calculations, we estimated the interband transition matrix element in Cf0 ðxp Þ [Eq. (4)] from the equation f hk3 =4srad jdz j2 ¼ 3 ex according to Hanamura’s general theory of the exciton radiative decay in spatially conﬁned systems [43], where srad h=E with ex is the exciton intrinsic radiative lifetime, and k ¼ 2pc E being the exciton total energy given in our case by Eq. (3). For zigzag-type CNs we here consider, the ﬁrst Brillouin zone of the lonh=3b 6 hkz 6 2p h=3b gitudinal quasi-momentum is given by 2p [1,2]. The total energy of the ground-internal-state exciton can h=3bÞ2 t2 =2Mex with 1 6 t 6 1 then be written as E ¼ Eexc þ ð2p representing the dimensionless longitudinal quasi-momentum. In our calculations we used the lowest bright exciton parameters and 19:1 ps, Eexc ¼ 1:21 eV and 1:00 eV, srad ex ¼ 14:3 ps Mex ¼ 0:44m0 and 0:19m0 (m0 is the free-electron mass) for the (11, 0) CN and (10, 0) CN, respectively, as reported in Ref. [25] by directly solving the Bethe–Salpeter equation.

664

I.V. Bondarev et al. / Optics Communications 282 (2009) 661–665

Fig. 4. (a) and (b) Exciton absorption lineshapes as the exciton energies are tuned to the nearest plasmon resonance energies (vertical dashed lines here; see Fig. 3, left panels) in the (11, 0) and (10, 0) CN, respectively. Dimensionless energy is deﬁned as ½Energy=2c0 , according to Eq. (2).

Both graphs in the right panels in Fig. 3 are seen to demonstrate a clear anticrossing behavior with the (Rabi) energy splitting 0.1 eV. This indicates the formation of the strongly coupled surface plasmon–exciton excitations in the nanotubes under consideration. It is important to realize that here we deal with the strong exciton–plasmon interaction supported by an individual quasi-1D nanostructure – a single-walled (small-diameter) semiconducting carbon nanotube, as opposed to the artiﬁcially fabricated metal– semiconductor nanostructures studied previously [29–31] where the metallic component normally carries the plasmon and the semiconducting one carries the exciton. It is also important that the effect comes not only from the height but also from the width of the plasmon resonance as is seen from the deﬁnition of the F p factor in Eq. (9). In other words, as long as the plasmon resonance is sharp enough (which is always the case for interband plasmons), so that the Lorentzian approximation Eq. (7) applies, the effect is determined by the area under the plasmon peak in the DOS function Eq. (5) rather then by the peak height as one would expect. We are now in a position to derive the exciton absorption lineshape function. To do that, we follow the optical absorption lineshape theory that one of us developed recently for atomically doped CNs [5]. In doing so, we take into account the exciton–phonon scattering in the relaxation time approximation. The (dimensionless) exciton absorption lineshape function IðxÞ in the vicinity of the plasmon resonance is then of the form

IðxÞ ¼

I0 ðxp Þ½ðx ef Þ2 þ Dx2p 2

½ðx ef Þ X 2f =42 þ ðx ef Þ2 ðDx2p þ De2f Þ

;

ð10Þ

pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ where I0 ðxp Þ ¼ Cf0 ðxp Þqðxp Þ=2p, X f ¼ 4pDxp I0 ðxp Þ, and Def ¼ h=2c0 sph ð< Dxp Þ is the exciton energy broadening due to the pho non scattering with the relaxation time sph . The calculated exciton absorption lineshapes for the CNs under consideration are shown in Fig. 4a and b as the exciton energies are tuned to the nearest plasmon resonances. We used sph ¼ 30 fs as reported in Ref. [17]. The line (Rabi) splitting effect is seen to be 0.1–0.3 eV, indicating the strong exciton–plasmon coupling with the formation of the mixed surface plasmon–exciton excitations. The splitting is larger in the smaller diameter nanotubes, and is not masked by the exciton–phonon scattering. Thus, we have shown the strong exciton–surface-plasmon coupling effect with the characteristic exciton absorption line (Rabi) splitting 0.1–0.3 eV in small-diameter ([1 nm) semiconducting CNs. This is almost as large as the typical exciton binding energies in such CNs (0.3–0.8 eV [9–11,14]), and of the same order of magnitude as the exciton–plasmon Rabi splitting in organic semiconductors (180 meV [29]). Also, this is much larger than the exciton–polariton Rabi splitting in semiconductor microcavities (140–400 leV [44–46]), or the exciton–plasmon Rabi splitting

in hybrid semiconductor–metal nanoparticle molecules [30]. However, the formation of the strongly coupled exciton–plasmon states is only possible if the exciton total energy is in resonance with the energy of an interband surface plasmon mode. The exciton energy might be tuned to the nearest plasmon resonance in ways used for the excitons in semiconductor quantum microcavities – thermally (by elevating sample temperature) [44–46], and/or electrostatically [47–50] (via the quantum conﬁned Stark effect with an external electrostatic ﬁeld applied perpendicular to the CN axis). The two possibilities inﬂuence the different degrees of freedom of the quasi-1D exciton – the (longitudinal) kinetic energy and the excitation energy, respectively [see Eq. (3)]. In the latter case, plasmon and exciton resonances both shift to the red due to the decrease in Eg as the ﬁeld increases [48]. However, the exciton shift is approximately twice as less due to the decrease in jEb j (see Ref. [48]), which is enough for the resonance to occur in view of the large jEb j contribution 0:5Eexc in small-diameter CNs [9–11,14]. This effect may be used for the development of CN based tunable optoelectronic device applications in areas such as nanophotonics and cavity quantum electrodynamics. Acknowledgements The work is supported by NSF (Grant Nos. ECS-0631347 and HRD-0833184). K.T. and L.M.W. are supported by DOE (Grant No. DE-FG02-06ER46297). I.V.B. acknowledges fruitful discussions with Alexander Govorov and Jonathan Finley. References [1] R. Saito, G. Dresselhaus, M.S. Dresselhaus, Science of Fullerens and Carbon Nanotubes, Imperial College Press, London, 1998. [2] H. Dai, Surf. Sci. 500 (2002) 218. [3] L.X. Zheng, M.J. O’Connell, S.K. Doorn, X.Z. Liao, Y.H. Zhao, E.A. Akhadov, M.A. Hoffbauer, B.J. Roop, Q.X. Jia, R.C. Dye, D.E. Peterson, S.M. Huang, J. Liu, Y.T. Zhu, Nat. Mater. 3 (2004) 673. [4] R.H. Baughman, A.A. Zakhidov, W.A. de Heer, Science 297 (2002) 787. [5] I.V. Bondarev, B. Vlahovic, Phys. Rev. B 74 (2006) 073401. [6] I.V. Bondarev, B. Vlahovic, Phys. Rev. B 75 (2007) 033402. [7] G.-H. Jeong, A.A. Farajian, R. Hatakeyama, T. Hirata, T. Yaguchi, K. Tohji, H. Mizuseki, Y. Kawazoe, Phys. Rev. B 68 (2003) 075410. [8] G.-H. Jeong, A.A. Farajian, T. Hirata, R. Hatakeyama, K. Tohji, T.M. Briere, H. Mizuseki, Y. Kawazoe, Thin Solid Films 435 (2003) 307. [9] T. Pedersen, Phys. Rev. B 67 (2003) 073401. [10] T. Pedersen, Carbon 42 (2004) 1007. [11] R.B. Capaz, C.D. Spataru, S. Ismail-Beigi, S.G. Louie, Phys. Rev. B 74 (2006) 121401. R. [12] C.D. Spataru, S. Ismail-Beigi, L.X. Benedict, S.G. Louie, Phys. Rev. Lett. 92 (2004) 077402. [13] F. Wang, G. Dukovic, L.E. Brus, T.F. Heinz, Phys. Rev. Lett. 92 (2004) 177401. [14] F. Wang, G. Dukovic, L.E. Brus, T.F. Heinz, Science 308 (2005) 838. [15] A. Hagen, M. Steiner, M.B. Raschke, C. Lienau, T. Hertel, H. Qian, A.J. Meixner, A. Hartschuh, Phys. Rev. Lett. 95 (2005) 197401. [16] F. Plentz, H.B. Ribeiro, A. Jorio, M.S. Strano, M.A. Pimenta, Phys. Rev. Lett. 95 (2005) 247401.

I.V. Bondarev et al. / Optics Communications 282 (2009) 661–665 [17] V. Perebeinos, J. Tersoff, Ph. Avouris, Phys. Rev. Lett. 94 (2005) 027402. [18] M. Lazzeri, S. Piscanec, F. Mauri, A.C. Ferrari, J. Robertson, Phys. Rev. Lett. 95 (2005) 236802. [19] S. Piscanec, M. Lazzeri, J. Robertson, A. Ferrari, F. Mauri, Phys. Rev. B 75 (2007) 035427. [20] S. Zaric, G.N. Ostojic, J. Shaver, J. Kono, O. Portugall, P.H. Frings, G.L.J.A. Rikken, M. Furis, S.A. Crooker, X. Wei, V.C. Moore, R.H. Hauge, R.E. Smalley, Phys. Rev. Lett. 96 (2006) 016406. [21] V. Perebeinos, Ph. Avouris, Nano Lett. 7 (2007) 609. [22] I.V. Bondarev, H. Qasmi, Physica E 40 (2008) 2365. [23] L.D. Landau, E.M. Lifshits, The Classical Theory of Fields, Pergamon, New York, 1975. [24] T. Pichler, M. Knupfer, M.S. Golden, J. Fink, A. Rinzler, R.E. Smalley, Phys. Rev. Lett. 80 (1998) 4729. [25] C.D. Spataru, S. Ismail-Beigi, R.B. Capaz, S.G. Louie, Phys. Rev. Lett. 95 (2005) 247402. [26] Y.-Z. Ma, C.D. Spataru, L. Valkunas, S.G. Louie, G.R. Fleming, Phys. Rev. B 74 (2006) 085402. [27] K. Kempa, P.R. Chura, in: L. Liz-Marzan, M. Giersig (Eds.), Special edition of the Kluwer Academic Press Journal, 2002. [28] K. Kempa, D. Broido, C. Beckwith, J. Cen, Phys. Rev. B 40 (1989) 8385. [29] J. Bellessa, C. Bonnand, J.C. Plenet, J. Mugnier, Phys. Rev. Lett. 93 (2004) 036404. [30] W. Zhang, A.O. Govorov, G.W. Bryant, Phys. Rev. Lett. 97 (2006) 146804. [31] Y. Fedutik, V.V. Temnov, O. Schöps, U. Woggon, M.V. Artemyev, Phys. Rev. Lett. 99 (2007) 136802. [32] I.V. Bondarev, Ph. Lambin, Phys. Rev. B 70 (2004) 035407; I.V. Bondarev, Ph. Lambin, Phys. Lett. A 328 (2004) 235.

665

[33] I.V. Bondarev, Ph. Lambin, Phys. Rev. B 72 (2005) 035451; I.V. Bondarev, Ph. Lambin, Solid State Commun. 132 (2004) 203. [34] I.V. Bondarev, Ph. Lambin, in: Trends in Nanotubes Research, Nova Science, NY, 2006, pp. 139–183 (Chapter 6). [35] S. Tasaki, K. Maekawa, T. Yamabe, Phys. Rev. B 57 (1998) 9301. [36] V.N. Popov, L. Henrard, Phys. Rev. B 70 (2004) 115407. [37] M.F. Lin, D.S. Chuu, K.W.-K. Shung, Phys. Rev. B 56 (1997) 1430. [38] H. Ehrenreich, M.H. Cohen, Phys. Rev. 115 (1959) 786. [39] T. Ando, J. Phys. Soc. Jpn. 74 (2005) 777. [40] X. Blase, L.X. Benedict, E.L. Shirley, S.G. Louie, Phys. Rev. Lett. 72 (1994) 1878. [41] K. Kempa, Phys. Rev. B 66 (2002) 195406. [42] W. Vogel, D.-G. Welsch, Quantum Optics, Wiley-VCH, NY, 2006. p. 337 (Chapter 10). [43] E. Hanamura, Phys. Rev. B 38 (1998) 1228. [44] J.P. Reithmaier, G. Se ß k, A. Löfﬂer, C. Hofmann, S. Kuhn, S. Reitzenstein, L.V. Keldysh, V.D. Kulakovskii, T.L. Reinecke, A. Forchel, Nature 432 (2004) 197. [45] T. Yoshie, A. Scherer, J. Hendrickson, G. Khitrova, H.M. Gibbs, G. Rupper, C. Ell, O.B. Shchekin, D.G. Deppe, Nature 432 (2004) 200. [46] E. Peter, P. Senellart, D. Martrou, A. Lemaître, J. Hours, J.M. Gérard, J. Bloch, Phys. Rev. Lett. 95 (2005) 067401. [47] D.A.B. Miller, D.S. Chemla, T.C. Damen, A.C. Gossard, W. Wiegmann, T.H. Wood, C.A. Burrus, Phys. Rev. Lett. 53 (1984) 2173. [48] D.A.B. Miller, D.S. Chemla, T.C. Damen, A.C. Gossard, W. Wiegmann, T.H. Wood, C.A. Burrus, Phys. Rev. B 32 (1985) 1043. [49] A. Zrenner, E. Beham, S. Stuﬂer, F. Findeis, M. Bichler, G. Abstreiter, Nature 418 (2002) 612. [50] H.J. Krenner, E.C. Clark, T. Nakaoka, M. Bichler, C. Scheurer, G. Abstreiter, J.J. Finley, Phys. Rev. Lett. 97 (2006) 076403.